Morphological characterization of Brazilian organ clays using AFM and SEM studies
International Journal of Modern Engineering Research (IJMER)www.ijmer.com Vol. 3, Issue. 3, May.-June. 2013 pp-1454-1457 ISSN: 2249-6645www.ijmer.com 1454 | PageA. Tejedor De León1, G. Navarro2, J. Rubio21Depto de Materiales y Metalurgia, Centro Regional de Veraguas – Universidad Tecnológica de Panamá2Laboratorio de Processamento Mineral – Depto. de Metalurgia – Universidade Federal do Rio Grande doSul - Brasil3Laboratorio de Tecnologia Mineral e Ambiental – Escola de Engeharia – Universidade Federal do RioGrande do Sul - BrasilABSTRACT: A combination of SEM (Scanning Electron Microscopy) and AFM (Atomic Force Microscopy)techniques was used to characterise the morphology of Brazilian montmorillonites before and afterintercalation of some organic compounds. AFM revealed that the layers are staked over above the others. Thesurface of the particles consisted of layers bounded with smooth flat basal planes and larger edges ending insome cascade-like steps 184 µm wide. Some micro and macro valleys (0.6 µm deep) are distributed throughoutthe whole area and irregularities on basal planes may be attributed to the crystallographic conditions of thegenesis of these Brazilian montmorillonites. The mapping performed over 20 x 40 areas showed adhesion forcesof 11 nN magnitude on bare clay mineral in the Na+ form and 40 nN for the calcium form. Forces between 10and 6 nN were found after organic intercalation. In general, the intercalation caused significant changes in thesurface properties of clay mineral. The combination of AFM and SEM studies provided evidence about the poorlcrystallinity of the Brazilian montmorillonites.Keywords: Atomic Force Microscopy, organoclays, montmorillonites, Scanning Electron Microscopý Volume3, Issue 2, Mar. – Apr. 2013.I. INTRODUCTIONAlthough the production of modified montmorillonites by the intercalation of organic compounds hasbeen recognised in many areas [1-4], little is known about the influence on its morphology.The morphology of clay mineral was studied by electron microscopy   and these studies revealed amultiplicity of microsteps on the clay mineral surfaces.Atomic Force Microscopy  has rapidly spread throughout many fields of science [8-10]  due to itshigh versatility. While height images provided quantitative topographic information, deflection images oftenrevealed finer surface details. The AFM can also record the force felt by the cantilever as the probe tip isbrought close to - and even into - a surface and then pulled away . This technique can be used to measurelong range attractive or repulsive forces between the probe tip and the surface, elucidating local chemical andmechanical properties and even the thickness of adsorbed molecular layers or bond rupture lengths .The aim of this work was to characterise the surface morphology of a Brazilian motmorillonite in thecalcium and sodium form and after intercalation of two organic compounds using a combination of SEM andAFM techniques.II. MATERIALS AND METHODS2.1 MaterialsBRASGEL, an industrial Brazilian montmorillonite in Na1+form Campina Grande – Paraiba, Brazil,BENTOCAL, a montmorillonite saturated with calcium cations. The organoclays used in these studies (FENANand ETIL) was obtained by the intercalation of two organic compounds, 1.1 ortho phenantroline andEthylenediamine respectively.2.2 Atomic force microscopy studiesThe morphological structure of different montmorillonites samples and its contact force curve were determinedby AFM by the contact mode (Digital Nanoscope IIIa, 3000 system, Si3N4 micro cantilever). The force curveobtained for each bentonite sample was utilised to calculate the nominal contact force of the tip on the surfacesamples, defined by the equations:F = kz (1)z = ADP (2)where: F = Contact force in nN; k = spring constant of the micro cantilever, 0.6 Nm-1; z = distancefrom de control point, nm; A = number of divisions of the cantilever deflection; D = potential applied,V/divisions; P = piezo sensitivity constant, 2 nmV-1.Morphological characterization of Brazilian organ clays usingAFM and SEM studies0204060801001st Qtr 2nd Qtr 3rd Qtr 4th QtrEastWestNorth
International Journal of Modern Engineering Research (IJMER)www.ijmer.com Vol. 3, Issue. 3, May.-June. 2013 pp-1454-1457 ISSN: 2249-6645www.ijmer.com 1455 | Page2.3 Scanning electron microscopy studiesSEM studies were performed with a Phillips XL-30 ESEM scanning microscope operating normally with up to30 kV acceleration voltage field emission gun. The samples were attached to a metal mount by carbon tape. Dueto the insulating nature of the materials, the samples were coated with a 20 nm thick layer of gold (Balzer UnionSCD 040 Sputter Coater system under argon vacuum.)III. RESULTS AND DISCUSION3.1 Topographical analysisThe nanotopography of BRASGEL sample is shown in Figure 1.Figure 1: Contac Mode Atomic Force Microscopy (CM-AFM) images of sodium Brazilian montmorillonite(BRAGEL)The 3D images of the sample, obtained by AFM studies, show different topography at various levels.The surface of BRASGEL shows complex morphological features with irregular and elongated edges, well-defined “hills” and several depressions, suggesting a surface with great roughness; the edges of the flakes, notclearly defined, are ragged and irregular. It also shows a successive “mountain range” with intermittent microand macrovalleys (~ 0.6 µm deep). This observation may be linked to a poorly crystallisation conditions whereby the Brazilian bentonites were formed .Figure 2 for the Ca-montmorillonite (BENTOCAL) shows the presence of a large jagged and an irregular edgeand an isolated volcano (~184 nm height )in the surface.Figure 2: AFM micrographs from the surface of BENTOCALIn the middle of the figure appears a defect caused by the tip – tip artefacts during image acquisition.Nevertheless microvalleys and grooves are seen (arrow marks). The surface is continuous and appears smooth.Also seen are the cascade.-like step structures, 280-345 nm wide as described by  who studied thenanomorphology of well and poorly crystallized kaolinites.Figure 3 obtained after Phenanthroline intercalation shows an apparently smooth surface unlike thenon-treated montmorillonite.
International Journal of Modern Engineering Research (IJMER)www.ijmer.com Vol. 3, Issue. 3, May.-June. 2013 pp-1454-1457 ISSN: 2249-6645www.ijmer.com 1456 | PageFigure 3: AFM micrographs on well-ordered montmorillonite after phenanthroline intercalation (FENAN)The overall topography is relatively regular and the basal planes are staked one above the other. Thesurface topography of the organoclay became smoother and presented a massive cascade-like structure at thelayer edges.Figure 4 shows a typical F-E (force vs. extension) curve obtained on the BRASGEL surface. The the slope ofthe curve suggests that the tip moved on a hard surface, and a typical large adhesion interaction curve wasrepresented .Figure 4: Computing contact force obtainen by AFM to the BRASGEL montmorillonite.The force curve represents the deflection signal for each complete trace-retrace cycle of the piezo. Atpoint a, the cantilever is not deflected but due to attractive forces between the tip and the bentonite surface, thetip sticks to the sample, and the cantilever is pulled down as the piezo continues to retract. Eventually, the springforce of the bent cantilever overcomes the attractive forces, and the cantilever quickly returns to its non-deflected, non-contact position. This is represented by point c. At point b, the spring force of the cantileverequals the attractive forces between the tip and the surface. The indentation in the surface was extremely“rough” (677.32 nm) and the extension of the sample was in the range of 5 x 5 m. The contact forces for theother samples were calculated by employing equations 1 and 2 (Table 1).Table 1: Contact forces onto Brazilian motmorillonites.Samples Resulting conctac force, nNBRASGEL 11BENTOCAL 40FENAN 10ETIL 6The BRASGEL sample presents an attactive contact force of 11 nN, between the sodium motmorillonite surfaceand the silicon nitride tip. In the case of alcium montmorillonite (BENTOCAL) the force increased to 40 nN.After the intercalation of Orthophenanthroline and Ethylenediamine the significantly reduced.
International Journal of Modern Engineering Research (IJMER)www.ijmer.com Vol. 3, Issue. 3, May.-June. 2013 pp-1454-1457 ISSN: 2249-6645www.ijmer.com 1457 | Page3.2. Micro structural analysisThe SEM image of BRASGEL bentonite shows a continuous surface, even though it contains small particlesand the edges of the lamellar are jagged and irregular (Fig. 5). The presence of a greater number of smaller sizeparticles between the lamellar make the sample less compact and less rigid (Frost et al., 2002). The formpresented by the Brazilian bentonites, is a typical “terraces landform” Figure 5: SEM micrographs of the motmorillonite (sodium form) - BRASGELIV. CONCLUSIONSThe results of these studies reveal that AFM and SEM are important complementary tools whileinvestigating clay mineral surfaces.Intercalation of EP and OP molecules caused a significant change in the surface properties of theBrazilian montmorillonite.The correlation between the AFM and SEM studies provided information about the poor crystalline ofthe Brazilian bentonite particles which, despite the poor crystallinity, the bentonites were very easy to graftedwith OP.The resulting OP organoclays shown more stability in terms of the resulting contact force performed inthe sequence works: intercalation, copper ions adsorption and desorption experiments than the bentonitesgrafted with ET.ACKNOWLEDGEMENTSThe authors are grateful to UTP (Panama), UFRGS (Brazil) and to the University of Nevada, Reno, Nevada,(USA) for technical support. Bentonit União Nordeste S.A. is also thanked for the supply of the bentonite claysamples.REFERENCES De León, A.T.; Nunes, D.G. and Rubio, J. Adsorption of Cu ions onto a 1.10 phenanthroline-grafted Brazilian bentonite. Clays andClay Minerlas. 1, 2003, 58 -64. Krishna, B.S.; Murty, D.S.R.; Jai Prakash, B.S. Surfactant-modified clay as adsorbent for chromate. Applied Clay Science. 20, 2001,65-71. Mortland, M.M.; Berkheiser, V. Triethylene diamine-clay complexes as matrices for adsorption and catalytic reactions. Clays andClay Minerals. 24, 1976, 60-63. Cox, M.; Rus-Romero, J.R.; Sheriff, T.S. The application of montmorillonite clays impregnated with organic extractants for theremoval of metals from aqueous solution Part I. The preparation of clays impregnated with di-(2-ethylhexyl) phosphoric acid andtheir use for the removal of copper (II). Chemical Engineering Journal. 84, 2001. 107-113. Zbik, M.; Smart, R.St.C. Nanomorphology of kaolinites: comparative SEM and AFM studies. Clays and Clay Minerals. 46, 1998,153-160. Thompson, D.W.; Macmillan, J.J.; Wyatt, D.A. Electron microscope studies of the surface microstructures of layer-lattice silicates.Journal of Colloid and Interface Science. 82, 1981, 362-372. Binnig, G.; Quate, C.F.; Gerber, Ch. Atomic force microscope. Physical Review Letters. 56, 1986, 930-933. Senna, L.F.; Achete, C.A.; Simão, R.A.; Hirsch, T. Comparative study between the electrochemical behavior of TiN, TiCxNy andCrN hard coatings by using microscopy and electrochemical techniques. Materials Research. 4, 2001, 137-141. Oréfice, R.L.; Brennan, A. Evaluation of the interactions between polymeric chains and surfaces with different structures performedby an atomic force microscope. Materials Research. 1, 1998, 19-28. Ikai, A.; Afrin R.; Itoh, A.; Thogersen, H.C.; Hayashi, Y.; Osada, T. Force measurements for membrane protein manipulation.Colloids and Surfaces B: Biointerfaces. 23, 2002, 165-171. Gopinath, T.R.; Schuster, H-D.; Schuckmann, W.K. (1981). Modelo de ocorrência e gênese da argila bentonítica de Boa Vista,Campina Grande, Paraíba. Revista Brasileira de Geociências. 11, 1981, 185-192.